Casting since about 4000 BC … Ancient Greece; bronze statue casting circa 450BC Iron works in early Europe, e.g. cast iron cannons from England circa 1543
Outline <ul><li>Sand Casting, Investment Casting, Die Casting </li></ul><ul><li>Basics and countermeasures </li></ul><ul><li>Phase Change, Shrinkage </li></ul><ul><li>Heat Transfer </li></ul><ul><li>Pattern Design </li></ul><ul><li>Variations & Developments </li></ul><ul><li>Environmental Issues </li></ul>
Casting <ul><li>Readings; </li></ul><ul><li>Kalpakjian, Chapters 10, 11, 12 </li></ul><ul><li>Booothroyd, “Design for Die Casting” </li></ul><ul><li>Flemings “Heat Flow in Solidification” </li></ul>Note: a good heat transfer reference can be found by Prof John Lienhard online http://web.mit.edu/lienhard/www/ahtt.html
Sand Casting Description: Tempered sand is packed into wood or metal pattern halves, removed form the pattern, and assembled with or without cores, and metal is poured into resultant cavities. Various core materials can be used. Molds are broken to remove castings. Specialized binders now in use can improve tolerances and surface finish. Metals: Most castable metals. Size Range: Limitation depends on foundry capabilities. Ounces to many tons. Tolerances: Non-Ferrous 1/32 to 6 Add .003 to 3 , 3/64 from 3 to 6 . Across parting line add .020 to .090 depending on size. (Assumes metal patterns) Surface Finish: Non-Ferrous: 150-350 RMS Ferrous: 300-700RMS Minimum Draft Requirements: 1 ° to 5° Cores: 1 ° to 1 1/2° Normal Minimum Section Thickness: Non-Ferrous: 1/8 - 1/4 Ferrous: 1/4 - 3/8 Ordering Quantities: All quantities Normal Lead Time: Samples: 2-10 weeks Production 2-4 weeks A.S.A.
Sand Casting Mold Features Vents , which are placed in molds to carry off gases produced when the molten metal comes into contact with the sand in the molds and core. They also exhaust air from the mold cavity as the molten metal flows into the mold.
Investment Casting The investment-casting process , also called the lost-wax process, was first used during the period 4000-3500 B.C. The pattern is made of wax or a plastic such as polystyrene. The sequences involved in investment casting are shown in Figure 11.18. The pattern is made by injecting molten wax or plastic into a metal die in the shape of the object.
Investment Casting Description: Metal mold makes wax or plastic replica. There are sprued, then surrounded with investment material, baked out, and metal is poured in the resultant cavity. Molds are broken to remove the castings. Metals: Most castable metals. Size Range: fraction of an ounce to 150 lbs.. Tolerances: .003 to 1/4 .004 to 1/2 , .005 per inch to 3 .003 for each additional inch Surface Finish: 63-125RMS Minimum Draft Requirements: None Normal Minimum Section Thickness: .030 (Small Areas) .060 (Large Areas) Ordering Quantities: Aluminum: usually under 1,000 Other metals: all quantities Normal Lead Time: Samples: 5-16 weeks (depending on complexity) Production 4-12 weeks A.S.A. (depending on subsequent operations). Talbot Associates Inc.
Die Casting – Cold-Chamber Casting Cycle in cold-chamber casting: (1) with die closed and ram withdrawn, molten metal is poured into the chamber; (2) ram forces metal to flow into die, maintaining pressure during the cooling and solidification; and (3) ram is withdrawn, die is opened, and part is ejected. Used for higher temperature metals eg Aluminum, Copper and alloys
Die Casting – Hot-Chamber Casting Cycle in hot-chamber casting: (1) with die closed and plunger withdrawn, molten metal flows into the chamber; (2) plunger forces metal in chamber to flow into die, maintaining pressure during cooling and solidification; and (3) plunger is withdrawn, die is opened, and solidified part is ejected. Finished part is shown in (4).
Die Casting Description: Molten metal is injected, under pressure, into hardened steel dies, often water cooled. Dies are opened, and castings are ejected. Metals: Aluminum, Zinc, Magnesium, and limited Brass. Size Range: Not normally over 2 feet square. Some foundries capable of larger sizes. Tolerances: Al and Mg .002 /in. Zinc .0015 /in. Brass .001 /in. Add .001 to .015 across parting line depending on size Surface Finish: 32-63RMS Minimum Draft Requirements: Al & Mg: 1 ° to 3° Zinc: 1/2 ° to 2° Brass: 2 ° to 5° Normal Minimum Section Thickness: Al & Mg: .03 Small Parts: .06 Medium Parts Zinc: .03 Small Parts: .045 Medium Parts Brass: .025 Small Parts: .040 Medium Parts Ordering Quantities: Usually 2,500 and up. Normal Lead Time: Samples: 12-20 weeks Production: ASAP after approval.
High Melt Temperature <ul><li>Chemical Activity </li></ul><ul><li>High Latent Heat </li></ul><ul><li>Handling </li></ul><ul><li>Off-gassing </li></ul>Tungsten Carbide, WC, Silicon Carbide, SiC Molybdenum Alumina Al 2 O 3 Platinum, Pt Titanium, Ti IronFE, Plain Carbon Steels, low alloy, stainless Nickel, Ni Nickel Allows Cubic Zirconia, ZrO 2 Silicon, Si Copper, Cu, Bronze, Brass Aluminum Magnesium Zinc, Zn PTFE (Teflon) Tin, Sn HDPE Nylon Acetal 3000 ° C 0 ° C 1000 ° C 2000 ° C
Mold Filling Bernouli’s Equation: Reynold’s Number: <ul><li>Short filling times </li></ul><ul><li>Potential Turbulence </li></ul><ul><li>(see p. 273 … Kalpakjian </li></ul>h
And more… Figure 7.2.32 Omit outside bosses and the need for cores. (Courtesy of Meehanite Metal Corp.) Figure 7.2.35 Avoid using ribs which meet at acute angles. (Courtesy of Meehanite Metal Corp.)
Die Casting Solidification Time s Time to form solid part A
Time to cool part to the ejection temperature. (lumped parameter model) let i = T i + T sp - T mold T sp = H/Cp f = T eject - T mold Integration yields… Or for thin sheets of thickness “w”, “ sp” means superheat
Pattern Design <ul><li>Table 12.1 </li></ul><ul><li>Normal Shrinkage Allowance for Some Metals Cast in Sand Molds </li></ul><ul><li>Metal Percent </li></ul><ul><li>Gray cast iron 0.83 – 1.3 </li></ul><ul><li>White cast iron 2.1 </li></ul><ul><li>Malleable cast iron 0.78 – 1.0 </li></ul><ul><li>Aluminum alloys 1.3 </li></ul><ul><li>Magnesium alloys 1.3 </li></ul><ul><li>Yellow brass 1.3 – 1.6 </li></ul><ul><li>Phosphor bronze 1.0 – 1.6 </li></ul><ul><li>Aluminum bronze 2.1 </li></ul><ul><li>High-manganese steel 2.6 </li></ul>
Variations and Developments <ul><li>Continuous casting </li></ul><ul><li>Lost foam molding </li></ul><ul><li>3D Printing of Investment tooling </li></ul><ul><li>Direct printing with metal droplets </li></ul><ul><li>Uniform metal spray </li></ul>
Continuous casting ref AISI Steel from the electric or basic oxygen furnace is tapped into a ladle and taken to the continuous casting machine. The ladle is raised onto a turret that rotates the ladle into the casting position above the tundish. Referring to Figure 2, liquid steel flows out of the ladle (1) into the tundish (2), and then into a water-cooled copper mold (3). Solidification begins in the mold, and continues through the First Zone (4) and Strand Guide (5). In this configuration, the strand is straightened (6), torch-cut (8), then discharged (12) for intermediate storage or hot charged for finished rolling.